# The the9ry of multifractal elasticity: basic laws and constitutive equations ```Revista Mexicana de F&iacute;sica 42, No. 3 (1996) 343-354
The the9ry of multifractal elasticity:
basic laws and constitutive equations
ALEXANDER S. BALANKIN
Instituto
Tecnol&oacute;gico y de Estudios
Superiores de Monterrey
Camp1fs Estado de M&eacute;xico, M&eacute;xico 52629
Recibido el 18 de agosto de 1995; aceptado el 29 de enero de 1996
,
ABSTRACT.Two basic laws of multifractatelasticity &aacute;re formu}ated in g&eacute;ner'al form, leading to a
closed system of constitutive equations. This approach allows t&oacute;' exp}ain '&iacute;he elasticity of materials governed by multifractal and hookean med&iacute;anisms. It is also noted that for materials of pure
multifractal origin their elasti&iquest; behavior can be used to est&iacute;mate three first generalized dimensions
(metric, information, and correlation) of random (multifractal) microstructure. With the introduced new framework, classical formulas for rubber-like,and spring-like elasticity are derived as
well as constitutive equations for superelastic materials. The theoretical resultsreasonably agree
with.experimental data and computer simulations reported in the literature.
.
,&quot;
RESUMEN.Se formulan&quot;en forma;general dos leyes b&aacute;sicas de la elastfeidad multifractal, que conducena&gt;un sistema de ecuaciones constitutivas. Este m&eacute;todo permite explicar el comportamiento
el&aacute;stico de materiales gobernados por mecanismos multifractales y /tookeanos. Se discute que para
materiales de origen puramente multifractal, su comportamiento el&aacute;stico puede ser empleado para
estimar las dimensiones m&eacute;trica, de informaci&oacute;n y de correlaci&oacute;n de microestructuras estoc&aacute;sticas
(multifractales). En este nuevo marco de referencia, se derivan las f&oacute;rmulas cl&aacute;sicas d&eacute; elasticidad rubber-like y spring-like, as&iacute; como las ecuaciones constitutivas para materiales superel&aacute;sticos.
Los resultados te&oacute;ricos obtenidos coinciden razonab&Iacute;emente con los datos experimentales y con las
simulaciones computacionales reportadas en la literatura.
PACS: 03.40.Dz; 62.20.Dc; 64.30.+t
In the last ten years the theory of materials with randol!l (fraetal 01' multifraetal) mierostrueture has beeome an attraetive tapie in mechanies ando physics of sol&iacute;as [1-6].
Statistieal properties of a multifraetal are eharaeterized by a speetrum ofgeneralized dimensions
dq . Generally,
the generalized
dimens!pn
dq
= O is equal
to the metrie (fractal)
&lt;iimensionevaluated by means of the box-counting algorithm, i.e., do = dF, which for multifractal structureis greatcr than its topologieal
dimension dT, but smaller than;' 01'equal
&quot;,
to, the topologiealdimension d of the enveloping Euclidean spaee, i.e., dT &lt; dF ~ dj the
generalizeddimcnsion of arder q = 1 is equal to the,ii&iacute;form&aacute;tion dimension dI = d&iexcl; j and
the dimension
dq
=
2 is equal to the eorrelation
integr~l exponent
de
=
d2, algo called
eO&Iacute;'relation dimension. Acrogel, eolloidal aggregates, polymcrs, some types of composite
materials, porous media, cte. llave a multifractal structure in a' wide range of spatial scales
Lo &lt; L &lt; Lu [1-3].
ALEXANDERS/BAL~NKIN
~
~
~
.
IJ}&quot;'~'
f !ll,.teria1s'with plultifr&amp;ftaI, &Iacute;J&Uuml;t'
~ure:' 1t~elastiC'1ty'ot&quot; ~J1ergetic nature
ntinui&Uacute;n;'crystaIs, &quot;polYcrYStiUs';&quot;'
e
ased ol&Iacute;:tne generaU~;Hooke'8 la.wj
2) entropy eI~ticity(elastomers),
b~eponG&aacute;us~)an
statiSt!cS &lt;t&iacute;eleme~ts(mjcrofstru~t&uacute;re&iexcl; a&iexcl;&ntilde;YJ&gt;er':and sup~relas&Uuml;dty, which are described by usi&Iacute;lg plienomenologicaI:modelsfor elastic ~poientialj and 4) spring-li~e elast~city (191lgpoIymer Ch&aacute;irls, foamB, Borne~tru&lt;:~
bella
(elaSt
~,.~
.',&quot;
o&quot;
o~&quot;&quot;,
~
.
turaI composjtes,
et~.) b'
on tpe:em
eras' .
.,'
.' bas'~
o
Jric&aacute;I form~la fol: spril!g~~o;. '.' .::&quot;
In:th~ se~Qfour wo.
:,;gr~;yp~'of
fract.~elasticity;(seeaJso;r~iewg15,6
ogI
fr&aacute;Cf
&quot;o.
,
d multifr~a.t
.
,
,
.
sugieStiji'that::&iexcl;siheo:rqulti-
'.
e)l.&aacute;vior forUl~t&eacute;rialSwith&quot;.
.,aY
&quot;d~
,'~ ~&quot;&quot;Qr
41co~ '~h~
gidilJa
s oft&eacute;Ve,r.~l .~'deforn&iacute;att9h
ultifractaI
.
/~() ;pos~te&lt;l'P
structures.
--o :~.
'..0 .~
o,.
-&quot;'~;::,.,
.,'
-&lt;,o
o
lJi, 'thi~attic1e' we~&quot;giv
~''g~ri~&iexcl;&aacute;tdormulationJ~r t~t
l~!is o(~uiti.fractaI
&quot;
.!le
in ofeoii~tit&uuml;~iv~'fquatioI&Iacute;s;::,illO~.be s&ntilde;()\ynth~t
elast{~it '
tbe-.entr
- ike e
.&quot; super.,.and 4Y&iacute;&gt;erelasticit~;~(&quot;&iexcl;::'8pring-!r
tici~Yc.
aie
~he spj&lt;:ifi~&quot;
of the m~
al ~
.. .&iexcl;he.generalization
o&iacute; tlte d
oped&iacute;i.theory
\vhitili-elJm1&gt;i the multif&iexcl;'~
lid:
f&Iacute;u}d&eacute;Wo
es
.1s'a:ls~ di\$cUSSed.
&quot;0B_~la\vs of.&gt;reyersibledeformati~el~icin
'tOi'm&uuml;lat~ inthe
&gt;'
o
f&oacute;llt')ws:.&quot;&lt;
geneJ'aI'fo~mas
&quot;
&quot;,;c;&quot;~;&quot;&quot;':
1) ~When the~~emiil &iexcl;;
F&iexcl;s'&iacute;&iacute;ppliea
~Jormat&Iacute;lin8 ocC.urlength,scale
'.
~pends oJP,;
Th~;,:'Ut
o
valid,
obeys re&iacute;atioJi~'
o'
,
tp tn,e ap1J&eacute;&quot;.;ante oj ~,,~ unique
netOcharoc~tr&iquest;~~1
Ir this-Jawis
.~,
ttl'iiit't!laitic 'is'~jjio;ctiil;objed,
bellond;;~ain:chns~
length,llJh,icJ.',
th~LE~~;:2'&quot;,..,
.;,'
;
oo.&quot;
~,':
.
;; the secon9':l~w ott~9dyif&aacute;mics-it
o
..'
,
&quot;1
,F~.~
( )
'IJLF
. .&quot;~~~
,&deg;;
aw
t au,
J
;:~;f1ll-/
&quot;'&quot;'
&quot;
&quot;.,:':
as
C-i~ '
( )
)
'T,'-'1'
IJE;
&quot;o
foJlows i1lat)1&iacute;~ force
.&quot;C:&quot;&iexcl;:,
'~ &quot;'
,o&quot;'~;,~,,:;
,
(l}
T'
.
Tbe fi!8ftermon ,th~ right of Eq. (1) is,eyidently the energy component of internal, forces,~&quot;'and the secondter~s
is theentropic
coIBP&lt;:ment&quot;,o;,
&quot;,,'&quot;
2) The reversible !-eJorma~io'MQl multijractaa are homeom~rphi~;
,
,
,
:
,
affine.
It jadear that ah&deg;Inoe~orphi9 deform,ation(one-to-oneami ont&oacute;t
formatiori) does
not ~gethe
mettic'(fractaI) dimenl)ion,ofa deformed multifracta1..Moreover in Ref. (15]
it waSshown that thel'e are'
gesmthe inform&aacute;tion:land c&oacute;rrelation dimensions a.f.
t:eI&quot;'aJfi~etr&aacute;n~f&oacute;rmation'(
de
)~!:~f
mult,ifl'act'fsthl~t
ure,whi}ec.t~e limiti~~!alues
, ,
;:e;' &quot; ,~:::-:&quot;,
&quot;
tyP&eacute;s o'{elastic be.1ui,~' 'e'b&iexcl;.sed~&oacute;1i':;diff&eacute;rent1&gt;henom~&iacute;iologicaj-la\~
to dJft'ert(
ijutive equations.
'&quot;'&quot;' ,
&quot;,'&iexcl;;~':f., &quot;1~&quot;'&iexcl;':
,
,
&quot;
,
, ,2 1'he'~initiaI IOOtphology'Q.f&iacute;~muJt,
,'.
ta1r~
~
.,
344
',be
chaiact&eacute;Ozed;;,by
,~
oJ}e;or;&iquest;m~re:,.gtb:
sCalePara.IJ.1eteFS'Lior dOE!Sn&oacute;t have them~.
'the fitst casththe:.ct:.may&quot;ha~rphXsi:caJ
signific,an~esuch as characteristi~ d~~nsion of-blob~ in' a polymer, ch!&Uacute;'~teristic oSi2:Et'of
cells&quot; &deg;L
meandistantebetWeenineIu .'
&quot;',
QpipQSitematerial,
cbaracteristii:r&aacute;dius6f&lt;;9rrelations
in a
,: random network'and aerog&eacute;l, ,
foll~ivs from the'l&aacute;.w p'Ostul~ted,'abo~, onfY:one of the~set
of scaJe paramet&eacute;rs Li (or the\r invariantc&oacute;tnbiriation) depenas on,ctlie'ex&iacute;ernal forceS. If theinitiaJ
mllltifractaJ gttucture has nost&aacute;le pa.tain~teistken the physical r&ntilde;&eacute;ariing&oacute;f LF. is the'Characteristic
lengthabOve which deformations occur. ':
'
THE THEORY OF MULTIFRACTAL
345
ELASTICITY:...
'o&iacute; generalized dimension spectrum, e.g., doo and d_oo,after affine.transformation in general differ from those for initial multifractal structure. Therefore, if the second postulate
(law) is valid the metric, information, and cmrelation dimensions of deformed multifractal
structure are constant.
The mass density p of a material with multifractal microstructure generally depends
on the length scale,L . Dimensional&quot; analysis implies the following general' functional
relation:
,,
P=PoiJ!
~c LF
(
)
(L'L ) =POiJ!Ac,Af,
(2)
where W is a dimensionless function of its dimensionless arguments Ac = ~c/L and~Af =
LF / L; ~c is the correlation length of multifractal (micro)structure. It is well known that
within the bounded interval
LF ~'L...~
(3)
~c
+
the,mass density of multifractal structure p(L) obeys &aacute; power law beh&aacute;vior [3}'{According
to inequality(3) the secondargument of the dimensionlessfunctioniJ!(Ac, Af) is small
(.\f ~ 1); so that ati'the asymptotic self-similar state we can apply to the function iJ!a
sqaling (incomple'teself-similarity) representation 
P0F= PpX&iexcl;c~ 'IjJ(Ac),
Q= d
-
dF,
(4)
where 'dF is the fractal Emetric, box-counting) dimension'pf the multifractal ami 'IjJis a
dimensio&ntilde;alessfunction of ~'c; Notice that,p possessscaling behavior (4) in&quot;the initial'stat~
of the multifractal structure' as well aw&quot;after any deformation of this structure, but~c and
dF, generally speaking, may be differentbefore and after the deformation.
However, according to the first la~9f reversible deformations, only the characteristic
length LF changes after elastic (reversible) deformation of elastically isotropic multifractal,
so that ~c must be constant. Furthermore, elastic deformations &quot;are h&lt;:nueomorphic by
definition and thus do not change the metric dimension dF of the deformed multifractal,
.
so that the scaling expqnent
Q is algo constant.
By this means, the mass density of elastic multifractal structure arte! its reversible
(homeomorphic) deformation caused by different external force&sect; Fl and F2 is equal to
p(F&iexcl;) = POAfl'IjJ(Ac)~nd p(F2) = POAf2'IjJ(Ac),
respectively. Hence the ratio p(F&iexcl;)/ p(F2) is
Jlot &iexcl;dependent on neither the varia15le ICl~gthscale ? nor..the correlation length ~c and
scales as
.
&quot;
p(F&iexcl;)
p( F2)
=
Afl
-(): =
( )
Af2
LFl
( )
-():
= AFO:'
L F2 T=const
Q= d
-
dF,
(5)
i. e. the relation governing the change in the mass density p of elastically deformed multifractaJs is similar to the relation that governs the change in the ma,ss d~nsity because
346
ALEXANDER
S. BALANKIN
of the geometric change in the dimensionalities of (multi)fractal structure3 (within the
interval (3)!).
It immediately follows form Eq. (5) that under uniaxial tension (compression) the
change in the dimensionality .of multifractal structure in the direction of external force
Fx, which is Ax = Lx/Ix, is accompanied by the change in the lateral dimensionalities of
deformed multifractal structure in orthogonal directions of the surrounding d-space with
A&iexcl; = L&iexcl;/l&iexcl;,wherei = 1,2, ... , d - 1. The lateral deformations A&iexcl; are related to Ax = AF as
Ai = Al.
= A;Vf' = AFvF,
i = 2,3,
. . . , d,
(6)
where lIF is the transverse deformation exponent.4
Substituting (6) into Eq. (5) we obtain a = 1 - (d - l)vF, so that
lIF
~
In Al.
-
dF
--1
.
In AF - d - 1
(7)
Therefore, if the first postulate (law) is valid, the transverse deformation exponent lIF of
an elastically isotropic multifractal is defined uniquely by its metric dimension.5
The data of Table 1 demonstrate that the results of calculations by the analytical
formula (7) agree well with results of computer simulations of the elastic properties of twodimensional percolation networks near a percolation threshold (see algo the Appendix), as
well as with the experimental data for aerogel SiO2 (which were obtained in the studies of
the longitudinal and transverse elastic waves propagation), rubber, and a strongly twisted
nondeformable polymer filaments.
At the same time, it must be emphasized that Eqs. (5) and (7) are not valid for materials
obeying conventional Poisson's effect, or, what is equivalent, the generalized Hooke's law.
For such materials the correlation length (c is equal to the sample size in the direction of
applied external force, i.e., (c ==Lx; so that (c and
AC
=
Ac1
Ac2
=
(8)
~Cl
(C2
must change .after deformation. At the same time, for an elastic continuum Ar = O and
AF ==1, while for a regular elastic lattice Ar = a/ ao (a and ao are the interatomic distances
before and after elastic deformation, respectively) and AF = Ac.Hence, for materials
obeying Poisson's effect our first postulate is not valido
3 Notice tbat formerly this fact was postulated as the second'law (see, for example reviews [5,6]).
In fact, as is shown above, Eq. (5) is a direct consequence o&iacute; the first law and o&iacute; the homeomorphism
o&iacute; reversible de&iacute;ormations.
4 Notice tbat the exponent of lateral deformation~ lIF
-In A1./AF is equal to the Poisson's
=
ratio v = -.JiA22 - li7iAll - li only in the limit of infinitely small strains &eacute;:&iexcl;&iexcl;= ~
&laquo; 1.
At first glance, it is surprising that lateral deformations are independent of the detailed geometry of de&iacute;ormed multi&iacute;ractal. Notice, however, that similar situations (power law distributions
of stresses and strains with exponents which are a function only o&iacute; Poisson's ratio) are common
within singular problems in the classical theory o&iacute; the elastic continuum obeying tbe intermediate
asymptotic behavior (see, for example [17,18]).
5
THE THEORY OF MULTIFRACTAL
347
ELASTICITY:...
TABLE 1. Comparison o&iacute; Poisson's ratio v, calculated using analytical relationship (7), with the
computed values, based on two-dimensional elastic random networks, and with experimental data
&iacute;or aerogel SiOz, strongly twisted nonde&iacute;ormable polymerfilament, and rubber.
Properties
Two-dimensional random network
o&iacute; size L x L near the percolation
threshold
(~c - correlation
length)
L/~c
Connectedness o&iacute;
random network
Fra.ctal
dimension o&iacute;
elastic backbone
dF
~
I/F, Eq. (7)
Poisson's ratio
(results o&iacute;
numerical
simulation and
experimental
data)
-~
00
L/f.c ...,..o
Elasticity o&iacute;
network is
determined by
danglingbonds
Bonds,
determining
elasticity o&iacute;
network are
multiduplicated
Dimension o&iacute;
geodesic line,
dmin = 1.1.:i:0.02 dF = drb,
drb = 3/4 

0.1 :i: 0.01
-1/3
0.08 :i:0.04

-0.33
Strongly -twisted
nonde&iacute;ormable
filament
Rubber
Fractal cluster
Monomer
Polymer network
dF, measured by
smaH;angle
neutr&Oacute;n
scattering and
molecular
2.3:i: 0.1
Dimension o&iacute; red
bonds,
. dF= dmin,
Aerogel SiO2
:i: 0.01

Dimensiori o&iacute;
sel&iacute;-avoiding
random walk:
d.-a = 2 
=
dF
3.00 :i: 0.04
[25,26]
0.15:i: 0.05
O
0.50 :i: 0.02
0.12:i: 0.08

O

0.50 :i: 0.01

~-&lt;~
Furthermore, the.&quot;metric dimension of an elastic continuum as well as a r,egular elaStic
lattice (dp ==dq for all q), which can be considered as a limiting c&iexcl;;tsesfor multifr~~tal
structures, is equal to the topological dimension of structure dT; so that
- '&quot;
d,
dp =d{
-
1,
a=
O, dT = d
{ 1, dT = d -
(9)
1.
Now, it is easyto understand that in the case of an euclidean elastic structure obeying
generalized Hooke's law the dimensionless
function 1/Ip(Ac)
= 1/I(Ac1)/1/I(Ac2)scales
limit of infinitely small strains!) as
1/Ip
=
( )
~Cl
~C2
(in the
-f3
== Lx(F&iexcl;) -f3= Xc/,
(
Lx(F2)
)
(10)
where {J = 1 - (dT - l)v. The relation for the conventional Poisson's effect Ejj ,= l/En
(see footnote 4) may be derived by substitution of Eqs. (10) and (6) with dT = d in the
general relation (4).
Therefore, in the general case of an elastic multifractal structure, the lateral deformations of which are governed bythe combination of lateral deformations of the &Iacute;nultifractal
nature with those associated with the conventional Poisson's effect, the scalingrelation (5)
348
ALEXANDER S. BALANKIN
can be generalized into
p(F&iexcl;) - A-(d-dF)~{dT-I)v-1
p(F2)&quot;- F
k,G
.
(11)
It should be emphasized, that relation (11) is valid only in the limit of infinitesimally small
strains Cii = J!A~ - 11~'1!
Now, if a mtiltifractal structure possesses Poisson's effect with Ae = AF,the transverse
deformation exponent is equal to
d-dF
lIF=lI-
([
(12)
1'
This relation governs the lateral d&eacute;f&oacute;rpiation of the multifractal&quot;is&quot;w&eacute;ll as the Poisson's
nature.
Below we will corisid~r only the elastic multifractals'.reversible behavior, whicli&quot;'is governed by the two laws postul&aacute;ted above. The lateral deformations of such'a structure nave
apure metric origin (Ae ='1)6'and are governed by the metric dimensionof the structure
(see Eq. (7)).
Looking back at the two proposed.laws oheversible deformations for multifractal structures, we see that we need to know the changes in the &eacute;ntropy and;~internal energy as functions of deformations before the closed system of constitutive equ&aacute;tions can be obtained.
Using the definitions of the inf&oacute;rmation'and correlation d&Iacute;lpensions and theif scaling
properties [1,2] with'rehttions (1), (5) valid, it is easy to show that the changes in the
thermodynamic entropy ~S(Ai) and in the internal energy'U(Ad during the reversible
deformation 'o&iacute; an elastic mtiltifractal in d-:-dimensional splce can be represented in the
&quot;',
~~
w
T ~S
= -C2
(
t
~=l
A1r
- d) ,
(l3)
and
~U
= -Ct(A~C -
1),
ae = d - de,
(14)
respectively. Here CI and C2 are constants (noti&lt;;ethat parameters CI and C2 can algo be
determined for any detailed mod&eacute;l of the~structure ).
Substituting (13) and(14) into (1), and using relations (5)-(7) we can derive the relationships between external force Fi and relative deformations Ai of multifractal structure.
For example, in the case of uniaxial deformation (tension 01'compression) wf obtain
FI
= C2{dIAfr-1-
dddF - (d - l)]Aidr[dF/(d-I)-I]-1 -&quot;cIC2 (d - dc)Af-dC-I
,
.
}
.
(15)
6 It is pertinent to note that in th~ case AC = AF and 11= l/(d-l)
Eqs. (11), (12) are equivalent
to Eqs. (5); (7), so that all results considered below are algo valid in this more general 'case.
THE THEORY OP MULTIPRACTAL ELASTICITY:..,
349
According to the dbvious condition F(&gt;'i = 1) = O,it followsfreIDEq. (15) that
Cl
C2
=d dId
dp
&lt;d
- de -
(16)
P,
so that 7
Fl
= C2dl{&gt;.f&iexcl;-l -
[dp- (d - l)]&gt;'ld&iexcl;(dF/(d-l)-l]-,~- (d - dp&raquo;.f-dc-l}~
(17)
Thus behavior patterns of elastic m:ultifra&lt;;tals (for which&quot;two laws pdstulated above are
valid!) are completely determined by the metric, information, and correlation dimensions.
Moreover, it is easy to see that in the limit of infinit'ely small strains, Eqs. (17) and (7)
can be,generalize~ by using Eqs. (11) and (12).'
In the case of monofractal structure all generalized dimensions areequal to the. metric
(fractal) dimension, i.e., dq ==dF = dI = de , and Eq. (16) results in the equality
Cl
c-..2
(18)
= dFf...&quot;'
So that, Eq. (15) may be rewritten in the forro
Fl
= Cl
{'&gt;.fF-l
- [dF- (d - l)]&gt;'lvFdF;l - (d - dF&raquo;'1-l}.
(19)
The stress 0&quot;11is related to the force Fl (.xI) by obvious equation 9':11= Fl&gt;.t-a, wliich
by using Eqs. (7), (19) may be written in theform
0&quot;11
=
E
1+6vF+4v~
&quot; 1+4vF
[ (.xl
-1)-2vp(&gt;'1
-1-
2
2VF,-1)],
(20)
where E = ({)O&quot;11/8E:11)r
is the Young modulus.
It is easy to see that, within the limit ofinfinitesima}ly small strains, j&eacute;:lll = &quot;.jl&gt;.it- 11 &laquo;
1, Eq, (20) leads to its classic counterpart for elastic continuuin. Thus~ fOl'monofractal
structure we llave Cl = 2(1 + vv)C2 = (1'+ 6VF f 4&iexcl;)~')E. ,Similarly, we can derive the
relations O&quot;ij(&gt;'k)for n-axial deformation of an elastically isotropic monofractal in the d
space. The pure shear is essentially a biaxial loading under the stresses 1711ande0&quot;22such
that there is no change in length aloi\g{~econd direction, i.e., &gt;'2= 1 (see Ref. [2'0]).
Therelationships between the elastic moduli, i.e., Young'sm08ulus E,'she~r modulus
G, and balk modulus D, and Lam&eacute; cocffieicnts &gt;.,J.lof elastically isotropic(mono!)fractal,
-
7 In Re&iacute;s. [5,6] we llave conjectured that &iacute;or an elastic multi&iacute;ractal d&iexcl;(d dp) = de(d - de).
This conjecture was made in the spirit o&iacute; the Dirac's mani&iacute;est tlyit ~a physicallaw must possess
mathematical beauty&quot;. However, there is no experimental evidente in support o&iacute; thisconjecture.
In this sense the Eqs. (16) and (17) are more correct ~han the related equations in Re&iacute;s. [5,6].
350
ALEXANDER S. BALANKIN
which are derived by analogy to the derivation of the corresponding relationships in classical theory of elastic continuum , are the following:
E
B = d(d - dF)'
G = E(d - 1)
2dF '
2
B = &gt;.+ &quot;d/t.
(21)
Notice that these relations differ from those which were conjectured for elastic fractals by
Bergman and Kantor . On the other hand, substituting Eq. (7) in the Eqs. (21) we
obtain expressions that' for d 7&quot; 2 [nd d = 3 are identical to those for two- and threedimensional elastically isotropic continuum!
ClassicaLformulas for rub1{er-likeelasticity [~2]
E
= E3 (&gt;'l' -
&gt;'12),
(22)
&gt;'2 = &gt;'3 ==X&iexcl;;1/2(p= const),
may be -derived within a framework of Eqs. (17) and (5)-(7) for multifractals obeying
= d = 3,
dF
and
dI
= 2.
Notice that the condition dI = 2 is assoti~ed with the Gaussian statistics [7,23], which
is used in the classical models of rubber=&Iacute;ike el{tsticity , while' the equality dF = d = 3
is the condition of incompressibility (see Eq. (5~), which is algo assumed in the classical
theory .
In fact, however, calculations based onEq. (22), with the vatue of E adjusted by fitting, are in reasonable agreement with the experiments only in the range of relatively
small strains (&gt;'i &lt; 1.2) . Traditionally, the refinement of the relation (22) is;made by
phenomenological modifications of the entropic theory, 9r by using empirical mod,els for
the elastic potential [22,24]. At the same time, elastomers are known to llave fractal or
multifractal microstructure [3,25,26]. Therefore, it is natural to describe rubber elasticity
of polymers by using the results of the concept of multifractal elasticity discuss~d above.
Generally the generalized dimensions of polymer networks swelled in a good solvent
are within the range 2 &lt; dq ~ 3 [3,25,26]. Assuming in the first approximation that
dF
= dI = de
and substituting
Eq. (7) intp E,q. (19), we,obtain
the relationship
between
the nominal stress Fl and the strain factor &gt;'1In the case of uniaxial tension (compression)
of an elastomer in the following fo~m:
=
F
1
E
1 +6/JF +A/J~ {
&gt;.1+2//F
- 2 ~-1-2//F(1+&quot;:F)- ( 1- 2
1
/JF
1
/JF
&raquo; .-2//F
..
1
},
(23)
which was first derived in our work [7&iexcl;by other l11t1ans.8Notice, that behavior (23) differs
from (22) even in the limit of incO,mpressibly defOl:m&eacute;d materi~l,whcn Eq. (23) r~d&uacute;ces
to the formula
.
F2
..
-i.
E
&gt;.2 - &gt;.-2.5
=_
),
4.5 ( 1
1
.-
(24)
8 We emphasize that Eq. (23)' is a lil11itingcase o&iacute; the general equation (19),which gives a richer
set o&iacute; various behavior patterns.
~
THE THEORY OF~ULTIFRACTAL
ELASTICITY:...
351
obeying the experimentally established ~ymptotic (see Ref. )
El &lt;XA~,
when
Al&raquo;
1.
It was shown in Refs. [5-11] that thei~&quot;talculations based on Eq. (23) agree well with
experimental data.,for rubbers without any~adjustment of parameters&laquo; except E) right. up
to Al = 7.
The nonlinear stress-elongation asymptotic for superelastic networks ,
O&quot;U &lt;X A 1/3
1
,
P5)
is a special case of constitutive e,guations (17) and (7), which is valid for multifractal
structures possessing
.
for example dF =
dF + dI - d
= 1,
(26)
2, d ~ 3, dI = 4/3.
The basic relation of spring-like elas~icity [22V
E
= E(A -
1)
(27)
mar be algo derived from. (17) and (5)-(Z) in the case of multifractal structures for which
.
dF = dI = 2 (d = 3).
Furthermore, the pseudo-elastic, super-elastic, and l'!lbber-li~e behavi&oacute;r of alloys ,with
thermoelastic martensitic transformation  can bealso evaluated within a framework of
the multifractal theory'of elasticity.9
Hence the proper regard for the real morphology allows an adequate description for
the behavior of a reversible deformed material with fra&lt;;talormultilractal microstructure.
Considereg, examples revealed that two laws of reversible deformations' of multifractal
structure, which are postulated in preseIlt work, are valid at least for some classes of
materials with (multi)f~a~tal (micro)structure.
Wechope this work will stimulateexperimental research along this Hile. We expect that
these investigations will support our concept of multifractal elasticity. If so, experimental
data on elastic behaviorcan be used to estimate the metric, information, and correlation
dimensions of the (multi)fractal microstructure.
ACKNOWLEDGMENTS
Theauthor is grateful to G. Cherepanov for usefuI discu&sect;siol1s.The courtesy and suppor,t of
the st{l.ffal1d faculty of Materials Research Cel1ter at Mol1terrey Ul1iversity of Techl1010gy,
and especially, A. Bravo, are gratefully ackl1owledged.
9'This tapie will be considered in moredetails
in a forthcoming papel'.
&gt;;.
352
ALEXANDER S. BALANKIN
ApPENDIX
The percolating network i8 a fundamental ,model ,for describing geometric,!:l fe.l:tturesof
random systems [2,29]. There are two main,.kinds of percolating networks: &quot;Bite&quot; ano
&quot;bond&quot;. To create a site-percolating network,~~ach inteJ;,section (site) of an initially pre'pared d-dimensionallattice is occupied at random with probability p. Sites are conneCted
if they are adjacent along a principal direction. In a bond-percolation network, all sites
are initially!occupied ano, 150.ndsaJ:~&quot;occupied randomlYt;with probability p. At a critical
(different) concentration p = pc (pc algo depends on the dimension ano symmetry of
originallat&Iacute;ice), both site ano boqd percolation exhibit a single, infinite cluster spanning
all space.
-
When the occ&uacute;P&lt;1tionprobability pJs less than pc, there are only finite clusters, whereas
if p &gt; pc anDinfinite.cluster is pieseht as well as finite clusters. The cluster 'both at pc
ano away from pc are characterized by the nuniber of sites, s, in tHe cluster ano by the
radius of gyration, Rg(s), of the cluster. Over what distances are occupied sites connected?
The connect~dness length (c is defined ~s the average root mean square distance between
occupied sites that belong to the same ano finitf. cluster. This connecte~nes~le'9gth is ,algo
called the correlation length. The lower cutoff;lscale characterizi!lg the,percol&aacute;tion cluster
is the length a that forros the lattice spacip.g'oftl&Iacute;e origiriallaHice.
For the problem of the&quot;electric&aacute;J condut'tivity of ahndom resistor Iletw&oacute;rk ano transport
dynamic properties, anotller object isrelevant: th~ cc&quot;backbone&quot;of an ihfinite percolation
cluster .'Fhe backbone is definedas the network ofunblocked connected bonos, through
which one can go to infinity by at'least two nonintersectingpaths.
In 'bther worn::l~,tg&eacute;
backbone is a set of bonos, through which~ele&quot;ctric current would flow were a.votta~e
applied to the cluster at infinitely remote efectro'&lt;:les.:::rherest:;6r the Clu.st~ri~refhre&lt;l to
as a collection of &quot;dead&quot; 01'','d~ngling ends&quot;. A dangling end cah be&quot;disconne~ted&quot;fr&oacute;mthe
cluster by cutting a single bond. In random resistor network near~the p~rcolation threshold,
some bonos carry'the highest current. These bonos forro the set of single cohnected bonos
of the backhone. This set qfbond}3were called &quot;red bonds&quot; (when one red bond is c~ut,
the current flow stops). 'The rest of bonos of the backbone is the &quot;blue bonds&quot; (Blue
bonds carry current, btit when'a blue bond is cut, the resistance of the system only slowly
increases). Anbther important concept is the minimalor &quot;chemical&quot;,path between&quot;&quot;two
points of a backbone, which is the shortest path between th~ two points. The shortest
path between the sites i and' j realizes along the &quot;geodesic lipe&quot;&quot; ano 'cahb&eacute; d~fi'ned as
the minimal number of steps'by wliichwe can reach j from i, witlf'l'estriction to existing
paths between connected sites. This is termed the chemlcal distance Lche~ (notice'that it
is not the same as the linear length measurcd between the two points ano referred t&uacute; as
the &quot;Euclidean. distance&quot; ).
For any length scale L &raquo; (c, a percolating system is macroscopically horn&lt;fgeneous.
But for a ~ L ~ (c, the system possesses statistical scaleinvariance ano may be' referred
to:as afractal or&quot;multifractal object, all properties ofw.hich obey a power law dependehce
on its characteristic linear size L . For exampl~/the total mitn:ber of bonos (01' sites)
.
of the cluster scales as NcI '&quot;
Ldcl,
~
where del'Is' the fractal dimension of the cluster; the
total number of backbonc bonos scales as N'bb '&quot; V{bb; thg number of red bonos Nred
scales with L as Nred '&quot; LDrb. The chemica1 dimension dchem is d~fincd from the relation
THE THEORY OF MULTIFRACTAL
ELASTICITY:...
353
Nchem '&quot; L~h~;;' The chemical length scales with Las Lchem '&quot; L1min, where the fractal
dimension o&iacute; g&eacute;odesic line dmin is equalto the'l'{Ltio del dchem'
/
Recently, there has been a considerabl&eacute; interestin th&eacute; elasti&eacute;&quot; properties of percolat...
ing random networks [21,28]. It was found that for elastic prbblem the critical value of
occupation probability PCel diffe.rs from pc . For example, for percolation on the twodimensional triangular lattice pc = 0.3473, whereas PCel= 0.58 . Hence .the elastic
backbone which govemscelastic behavior of percolating network CaIgodiffers from backbone,govemed electrical resistance. Among the surprises tliat *were uncoyered was the
phenomenon
of a negative Poisson's
ratio'&Iacute;I
of percolation
network of size L &laquo;
~c near
the percolation threshold (L ~ a) . It was algo found that the Poisson's ratio is sensitive to the precise value of L/~c, changing from -0.33 when L/~c -+ O to about +0.08
when L/~c -+ 00 (a zero Poisson's ratio was found for L/~c ::=0.2)  The most im-
portant result of the refered works is that the limiting values of v (namely v(O) = -0.33
and v(oo) = 0.08) are independent of the elementary (microscopic) force constants of
the bonds. This give the rige to describe the elastic behavior of sutIl networks within a
framework of the theory of multifractal elasticity (see Table 1).
REFERENCES
1. T. Vicsek, Fractal Growth Phenomena, London, World Scientific(1992).
2. A.S. Balankin, Synergetics 01 Delormed Solids, Mos&eacute;ow, Department of Defense USSR press
(1991).
.
3. V.S. lvanova, A.S. Balankin, l.J. Bunin, andA.A. Oksogoev, Synergetics and Fractals in Material Sc&iacute;ence, Nauka,.Moscow (1994).
4. G.P. Cherepanov, A.S. Balankin and V.S. lvanova,. in A Topical Encycl()pedia 01 Current
Knowledge Dedicated Alan Arnold Griffith, Edited by G.P. Cherepanoy, Krieger, Melborne,
U.S.A. (1996),
5.
6.
7.
8.
9.
10.
11.
12.
13.
14.
15.
16.
17.
18.
19.
20.
21.
22.
23.
.
A.S. Balankin and P. Tamayo, Rev. Mex. F&iacute;s. 40 (1994)506.
G.P. Cherepanov, A.S. Balankin and V.S. IvanOva, Eng. Fracture Mech. 51 (1995) 997.
A.S. Balankin, Sov. Phys. Tech~ Lett. 17 (1991) 632.
A.S. Balankin, Dokl. Russian Academy 01 Sc&iacute;. 319 (1991) 1098.
A.S. Balankin, Sov. Phys. Dokl. 37 (1992) 379.
A.S. Balankin and A.L. Bugrimov, Polymer Sci. 34 (lQ92) 889.
A.S. Balankin and A.L. Bugrimov, in Abstr. XXVIII Int. Congr. Theor. and Ajipl. Mech.
Haila, Israel, August 22~28, 1992, lut. Union Theor. and Appl. Mech. Press, Haifa (1992) 17.
A.S. Balankin, Phys. Lett. A210 (1996) 51.
A.S. Balankin, Sov. Phys. Salid State 34 (1992) 658.
A.S. Balankin, Phys. Rev. B 53 (1996) 5438.
A.S. Balankin, J. Phys. A (in press).
G.l. Barenblatt, Similarity, sell-similarity and intermediate asymptotics, New York, Consultant
Buerau J1979).
G.P. Cherepanov, Mechanics 01 Composite Materials, Moscow, Nauka (1983).
A.S. Balankin, Sov. Tec~. Phys. Le~t. 175(1,,991)229; 391.
S.V. Panyukov, Sov. Phys. JETP71 (1990)\$372.
.
A.E.H. Love, A Treatise on the Mathematical Theory,pl ElO,st&iacute;c&iacute;ty, Dover, New York 01.944).
D.J. Bergman and Y. Kantor, Phys. Rev. Lett. 53 (lfJ84) 511.
L. Treloar, The Physics 01 R1,bber Elas.,tic&iacute;ty, Clarendom Press, Oxford (1975).
C.E. Puente, Phys. Lett. A 161 (1992) 441.
..~'&quot;
354
ALEXANDER
S.BALANKIN
24.~S. Edwards and T. Bilgis, Rev. Progr. Phys. 51 (1988) 243.
25. A:M. Aharoni, in Synthesis, Characterization, and Theory 01 Polymer Networks and Gels,
edited by ~~M. Aharoni, Plenum Press, New. York (1992).
26. M. Kallala, C. Sanchesand B. Cabane, Phys. Rev. E 48 (1993) 3692.
27.
28.
29.
30.
.
S.P. Obukhov, M. Rubinstein and R.H. Colby, Macromolecules 27 (1994) 3191.
E. Duering and D.J. Bergman, Phys. Rev. B 37 (1988) 9460.
M.B. Isichenko, Rev. Modern. Phys. 64 (1992) 961.
M. Gronauer, A. Kadur and J. Fricke, in Proc. 1st Symp. Aerogels, Wurzburg, Germany, 1985,
Springer- Verlag, Berlin (1986).
31. B.M. Smirnov, Physics 01 Fractal Clusters, Nauka, Moscow (1991).
32. S. Feng and P.N. SeD, Phys. Rev. Lett. 52 (1984) 216.
```